Hindawi Publishing Corporation
Advances in Civil Engineering
Volume 2012,Article ID391214,10 pages
doi:10.1155/2012/391214
Research Article
APrediction Method of Tensile Young’s Modulus of
Concrete at Early Age
Isamu Yoshitake,
1
Farshad Rajabipour,
2
Yoichi Mimura,
3
and AndrewScanlon
2
1
Department of Civil and Environmental Engineering,Yamaguchi University,Ube,Yamaguchi 7558611,Japan
2
Department of Civil and Environmental Engineering,Pennsylvania State University,University Park,PA 16802,USA
3
Department of Civil and Environmental Engineering,Kure National College of Technology,Kure,Hiroshima 7378506,Japan
Correspondence should be addressed to Isamu Yoshitake,yositake@yamaguchiu.ac.jp
Received 7 March 2011;Accepted 22 September 2011
Academic Editor:Kent A.Harries
Copyright © 2012 Isamu Yoshitake et al.This is an open access article distributed under the Creative Commons Attribution
License,which permits unrestricted use,distribution,and reproduction in any medium,provided the original work is properly
cited.
Knowledge of the tensile Young’s modulus of concrete at early ages is important for estimating the risk of cracking due to restrained
shrinkage and thermal contraction.However,most often,the tensile modulus is considered equal to the compressive modulus and
is estimated empirically based on the measurements of compressive strength.To evaluate the validity of this approach,the tensile
Young’s moduli of 6 concrete and mortar mixtures are measured using a direct tension test.The results show that the tensile
moduli are approximately 1.0–1.3times larger than the compressive moduli within the material’s ﬁrst week of age.To enable
a direct estimation of the tensile modulus of concrete,a simple threephase composite model is developed based on random
distributions of coarse aggregate,mortar,and air void phases.The model predictions show good agreement with experimental
measurements of tensile modulus at early age.
1.Introduction
An accurate estimation of the Young’s modulus is important
for proper structural design of concrete members,and ensur
ing their serviceability,such as controlling deﬂections and
crack widths.In particular,the timedependent development
of the tensile Young’s modulus at early ages is needed for
estimation of the tensile stresses that are generated due
to restrained thermal and hygral shrinkage.These tensile
stresses may lead to premature cracking of concrete mem
bers.Currently,the tensile modulus is assumed to be equal
in value to the compressive modulus and is estimated using
empirical correlations based on the compressive strength
of concrete [1,2].The Architectural Institute of Japan
(AIJ) [3] points out that employing the tensile modulus
is more appropriate for estimation of the risk of early
age cracking;however,the speciﬁcation indicates that the
compressive modulus may be used instead of the tensile
modulus because investigations dealing with the tensile
modulus are currently insuﬃcient.Since the tensile behavior
of concrete is more signiﬁcantly aﬀected by the presence of
ﬂaws (e.g.,microcracks or large capillary pores common in
earlyage concrete),it is important to develop tools to predict
or measure the tensile properties more accurately.
Direct tension tests have been conducted in earlier
studies to investigate the tensile strengthand the tensile strain
capacity of concrete.Although the tensile moduli can be
obtained fromthe linear portion of the stressstrain diagram
in these reports,the focus of these earlier studies has been
primarily on mature concrete.As such,little information
is available on the earlyage (i.e.,less than 28 days) tensile
modulus and its development with time.In addition,a
reliable model to aid design engineers in estimating the
tensile modulus based on concrete’s proportions and age
does not currently exist.
Xie and Liu [4] conducted a direct tension test using
small and large specimens of mature concrete with var
ious aggregate sizes,and measured the tensile strength,
strain capacity,and Young’s modulus.They observed that
increasing the maximum aggregate size does not have a
proportional impact on tensile strength and tensile modulus
of concrete.Oluokun et al.[5] researched the compressive
2 Advances in Civil Engineering
Young’s modulus and Poisson’s ratio of earlyage concrete.
They concluded that the compressive modulus is propor
tional to the 0.5 power of the compressive strength,and
the ACI 318 formula for estimation of the compressive
modulus is valid after the age of 12 hours.Hagihara et al.
[6] investigated the tensile creep of highstrength concrete
at early age,and reported that the tensile Young’s moduli
are approximately 15%higher than the compressive moduli.
This is an important conclusion and should be evaluated
for other concretes with normal strength.Swaddiwudhipong
et al.[7] investigated the mechanical properties of con
crete containing ground granulated blast furnace slag and
pulverized fuel ash.They reported that the tensile moduli
of all concretes tested had correlated well with the tensile
strength;although no predictive formula is presented for
the tensile modulus.Aoki et al.[2] also conducted direct
tension test in order to obtain tensile strength and Young’s
modulus of mature concrete and found that the tensile
modulus is 9–12% higher than the compressive modulus
for these concretes.Bissonnette et al.[8] researched the
tensile creep of concrete at early age,and presented some
measurements of the tensile Young’s modulus at the age of
7 and 28 days.In an earlier work [9],the authors investigated
the tensile Young’s moduli by using a direct tension test,
and presented a composite model derived from the Hirsh
model [10] to predict the tensile modulus.The model
showed good agreement with the experimental data as well as
other composite models oﬀered by Counto [11] and Hashin
[12].Recently,Mihashi and Leite [13] presented a state
oftheart report on early age cracking of concrete and its
mitigation techniques that includes some information on the
mechanical properties of concrete at early ages.
As described above,the investigations focusing on the
tensile Young’s modulus of earlyage concrete are few,and
more experimental data will be needed to establish reliable
predictive correlations for estimation of the tensile modulus.
The present paper reports laboratory measurements of the
tensile modulus within the ﬁrst 7 days of hydration.Three
concrete mixtures (with diﬀerent W/C) were tested.In
addition,to evaluate the eﬀect of aggregate size,duplicate
concrete mixtures were prepared and sieved before setting
using a 5 mm mesh sieve.The resulting mortars were
tested to determine their tensile Young’s modulus.Using the
measurements results,a composite model was developed and
calibrated which can serve as a simple method for estimating
the tensile Young’s modulus of concrete.
2.Experimental Program
2.1.Materials and Mix Proportions of Concrete.This study
employed ordinary Portland cement with a density of
3.14 g/cm
3
.Tables 1 and 2 provide the details of the cement
and aggregate used.Proportions of the six concrete and
mortar mixtures tested in this study are given in Table 3.
The proportions of the concrete were designed by referring
to mixture proportions used in a ready mixed concrete
plant in Japan.Mortars were obtained by sieving plastic
concrete mixtures as discussed above.This was done to
duplicate the mechanical properties (i.e.,tensile modulus)
Table 1:Physical and chemical compositions of cement.
Ordinary Portland cement
Density 3.14 g/cm
3
Blaine ﬁneness 3340 cm
2
/g
Setting time startend 2 h 26 m–3 h 34 m
Comp.strength at 3 days 30.8 MPa
at 7 days 46.3 MPa
at 28 days 63.6 MPa
Chemical compositions
CaO 64.5%
SiO
2
20.5%
Al
2
O
3
5.7%
Fe
2
O
3
2.9%
MgO 1.27%
SO
3
2.15%
Cl
−
0.009%
Loss of ignition 1.89%
Table 2:Properties of aggregate.
Fine agg.S Crushed rock G
Materials Sea sand Andesite
Density 2.56 g/cm
3
2.73 g/cm
3
Fineness modulus 3.36 6.66
Absorption 1.3% 1.3%
Size (max.– min.) 5 mm 20–5 mm
of the mortar portion of the concretes as closely as possible.
These results are needed to develop the composite model
as discussed in Section 3.In all mixtures,proper dosages of
air entraining and water reducing admixtures were used to
ensure consistency and workability of the concrete (Table 3).
2.2.Test Methods and Specimens.Figure 1 shows the direct
tension apparatus used in this study.Figure 2 shows the
geometry of the dogbone specimens tested.To reduce
bending moment during test,the ends of the dogbone
specimens were not fully ﬁxed but were allowed rotational
freedom.The direct tension apparatus manually provides
a tensile force to a specimen using a lever.Overall,an
approximately constant strain rate of 2 to 3
×
10
−
6
/sec
was applied.To measure tensile strain of specimens,an
embedded strain sensor was used which includes an electrical
resistance wire strain gage of 60 mm long coated by epoxy
resin with tensile modulus of 2.8 kPa as shown in Figure 2.
The overall sensor size was 120
×
10
×
3mm;as such the
area ratio of the sensor to concrete was smaller than 1.4%
to ensure that the sensor has little inﬂuence on the behavior
of specimens when subjected to tensile force.While this
setup was used to measure the tensile modulus,it may not
be suitable for measurement of the tensile strength since a
number of breaks occurred within the end zones of the dog
bone specimens (Figure 3).
Advances in Civil Engineering 3
Table 3:Mixture proportions of concrete.
ID W/C (%) Water (kg/m
3
) Cement (kg/m
3
) S (kg/m
3
) G (kg/m
3
) WRA (kg/m
3
) Air (%)
O57 57 165 290 812 1030 2.9 4.5
O57m
#1
57 265 466 1304 — 4.7 —
#2
O39 39 169 434 790 933 4.3 3.8
O39m
#1
39 257 659 1200 — 6.5 —
#2
O25 25 170 680 694 818 6.8 3.6
O25m
#1
25 243 971 991 — 9.7 —
#2
#1
Mortar is made fromwet screening of concrete (maximummesh size:5 mm).
#2
Air content of mortar was not measured because it is diﬃcult to obtain wetscreened mortar volume required for the test.
Chain Chain
Load cell
Load
Pin
Specimen
Grip
Lever
Figure 1:Direct tension test using a dogboneshaped specimen.
10
15 70 120 70 15
75 100
20 80 20
20
t
=
3
Epoxy resin Strain gage (60 mmlong)
(unit:mm,1 mm
=
0.0394 in.)
Sensor
Specimen
Sensor
Figure 2:A dogboneshaped specimen and an embedded sensor.
3.Prediction of the Young’s Modulus Using
a Composite Model
In addition to the tensile modulus,the compression and
indirect tension tests were conducted using cylindrical spec
imens.The compressive modulus of concrete was obtained
using an extensometer equipped with 2 displacement gages,
and the modulus of mortar was measured using 2 wire strain
gages 30 mm long.The cylindrical specimens (diameter
×
height) tested were 100
×
200mm for concrete,and 50
×
100mm for mortar.Three cylindrical specimens were used
for each test per each mixture,and the average of the three
measurements was used.The tests were performed at ages 1,
2,3,and 7 days.
3.1.Determination of the Tensile Young’s Modulus.To mea
sure the tensile modulus,the tensile force is applied to the
specimen at strain intervals of 10
×
10
−
6
.In order to prevent
failure of specimen,the maximumstrain during the test is set
at 60
×
10
−
6
.Since the plastic strain of concrete at early age
Figure 3:Typical failure within the end zone of the dogbone
shaped specimen.
Young’s modulus
Tensilestress(MPa)
×
10
−
6
1010 20 30
Strain at loading
Residual strain
Loading
Removing load
Tensile strain
Figure 4:Evaluation method for tensile Young’s modulus.
may comprise a high percentage of the total strain measured,
the tensile modulus is obtained fromthe unloading branches
of the stressstrain relation as shown in Figure 4.The slope
of the unloading branches after the specimen was loaded
to 10
×
10
−
6
,20
×
10
−
6
,and so forth,is determined and
averaged to obtain the tensile modulus of the specimen.The
force is measured twice at each strain level using a load cell
4 Advances in Civil Engineering
(Tension)
(Tension)
(Compression)
(Compression)
E
1
V
1
E
2
V
2
E
i
V
i
E
n
V
n
(a)
E
1
V
1
E
2
V
2
E
i
V
i
E
n
V
n
(Tension)
(Compression)
(Compression)
(Tension)
(b)
(Tension)
E
m
V
m
E
g
V
g
(Tension)
(Compression)
(Compression)
(c)
E
m
V
m
E
g
V
g
(Tension)
(Tension)
(Compression)
(Compression)
(d)
Figure 5:Typical composite models for predicting Young’s modulus:(a) Parallel model,(b) Series model,(c) Counto model,and (d) Hashin
model.
with an accuracy of 0.1 kNand capacity of 200 kN.As will be
discussed later,the maximumresidual strain after unloading
of each specimen was measured as 3
×
10
−
6
.In each case,
concrete and mortar specimens were made from the same
batch using the sieving procedure mentioned above.
As mentioned earlier,the tensile Young’s modulus of
concrete is often assumed to be equal in value to the
compressive modulus.In addition,the compressive modulus
of concrete is frequently estimated based on empirical corre
lations with concrete compressive strength.The compressive
modulus of concrete has also been related to the volume and
mechanical properties of concrete’s constituents (aggregates,
paste,etc.) using some classical composite models such
as those presented by Zhou et al.[14],Topc¸u [15],and
Yoshitake et al.[9].A brief overview of these models
is provided below.
The typical composite models for estimation of the
elastic modulus are illustrated in Figure 5.These include (a)
the Parallel model,(b) the Series model,(c) the Counto
model [11],and (d) the Hashin model [12];as represented
by the following:
Parallel model:E
=
n
i
=
1
E
i
∙
V
i
,
(1)
Series model:
1
E
=
n
i
=
1
V
i
E
i
,(2)
Advances in Civil Engineering 5
E
a
v
a
E
m
v
m
E
g
v
g
Parallel model
Seriesmodel
(Tension)
(Compression)
(Compression)
(Tension)
E:Young’s modulus of each material
v:volume of each element
a:air,m:mortar,g:coarse agg
E
m
v
m
Figure 6:An example of a simple composite model using parallel
and series models.
Counto model:
E
E
m
=
1 +
V
g
V
g
−
V
g
+E
m
/
E
g
−
E
m
,
(3)
Hashin model:
E
E
m
=
V
m
E
m
+
1 +V
g
E
g
1 +V
g
E
m
+V
m
E
g
,(4)
where E
i
and V
i
represent the Young’s modulus and the
volume fraction of concrete constituents (e.g.,mortar,coarse
aggregate,etc.),n is the number of constituents,and the
subscripts m and g refer to mortar and coarse aggregate,
respectively.The Counto and Hashin models are based on
a 2phase composite (mortar and aggregate).While these
models are generally more accurate than simple parallel and
series models,they may estimate the Young’s modulus inap
propriately for concretes containing high aggregate volumes
or high air content.
In the present work a new triphase model is proposed
based on random distribution of elements within a 2
dimensional 80
×
80 grid (Figure 6).Each element in
the model is composed of mortar,coarse aggregate,or
air.The number elements corresponding to each phase is
proportional to the volume fractionof that phase in concrete.
Elements are placed randomly in the model using a Monte
Carlo procedure.To determine the tensile modulus of the
grid,simple micromechanical calculations are performed
based on the series and parallel models.First the tensile
modulus of each row of elements is determined using
the parallel model and then the modulus of the grid is
determined by combining all rows using the series model.
Alternatively,the modulus of each column can ﬁrst be
determined using the series model and then the columns are
combined using the parallel model.
4.Experimental Results and Discussion
4.1.Evaluation of the Reliability of the Embedded Strain
Sensor.It is important to ensure proper measurements of
the tensile strain using the embedded strain sensor.For this
purpose,a dogbone concrete specimen is tested in tension
0
10
20
30
40
50
0 10 20 30 40 50
Surfacestrain
×
10
−
6
Surface strain
Inside strain
×
+
Inside strain
×
10
−
6
Figure 7:Comparison of inside strain and surface strain.
and the tensile strain is measured by both the embedded
gage as well as 2 wire strain gages mounted on the surface of
the concrete specimen.Figure 7 presents the results showing
that the internally measured strain is practically equal to the
surface measured strains.This implies that the tensile stress is
applied uniformly to the specimen and the embedded sensor
can be used to monitor concrete’s tensile strain.Based on this
conclusion,further measurements in this study employ only
the embedded sensor.
4.2.Tensile StressStrain Responses.Figure 8 presents exam
ples of the tensile stressstrain responses of each concrete.As
shown,the slope of each stressstrain regression line (i.e.,the
tensile modulus) develops with increasing age and reducing
the watercement ratio (W/C) of concrete.Figure 8(a) shows
the stressstrain response at 1 day;the results indicate that
the residual strain after unloading of specimens is zero (i.e.,
plastic strain at age of 1 day when specimen are loaded to
60
×
10
−
6
is negligible).Note that the response of mixture
O57 (W/C
=
57%) at 1 day could not be obtained because the
concrete was too weak to allowperforming the direct tension
test.Figure 8(b) presents the stressstrain responses at 7 days;
the maximumresidual strain after loading specimens to 60
×
10
−
6
is 3
×
10
−
6
corresponding to the mixture O39.For this
mix,had the loading branches of the stressstrain response
been used to determine the modulus,the tensile modulus
would be estimated as 31.2 GPa,comparing with 33.0 GPa
obtained from using the unloading stressstrain branches.
The ratio of the modulus obtained by the two methods is
approximately 0.95.
4.3.Time Dependent Development of the Mechanical Prop
erties.The results of the compressive and splitting tensile
strength measurements of the three concrete mixtures are
presented in Figure 9.At 7 days,the concrete mixtures have
compressive strengths in the range of 20 to 45 MPa,and
splitting tensile strengths in the range of 2 to 3.3 MPa.The
timedependent compressive and tensile Young’s moduli are
6 Advances in Civil Engineering
0
0.5
1
1.5
2
0 10 20 30 40 50 60 70
Tensilestress(MPa)
Strain
O39
O39
O25
O25
×
10
−
6
(a)
0 10 20 30 40 50 60 70
Tensilestress(MPa)
Strain
O57
0.5
1
1.5
2
0
O25
O39
O57
O39
O25
×
10
−
6
(b)
Figure 8:Tensile stressstrain responses:(a) age of 1 day and (b) age of 7 days.
0
10
20
30
40
50
0
1
2
3
4
5
0 1 2 3 4 5 6 7 8
ft
(MPa)
Age (day)
O57,tensileO57,compressive
O39,tensileO39,compressive
O25,tensileO25,compressive
f
c
(MPa)
Figure 9:Strengths versus age of concrete.
presented in Figure 10.The compressive moduli in the graph
demonstrate the secant moduli under 33%of the maximum
stress.Based on Figure 10,the tensile Young’s moduli are
approximately 1.0–1.3times larger than the compressive
moduli.The result may be caused by diﬀerent response
to stress applied to each specimen,such that the tensile
stresses were less than 10%of the compressive stresses.This
diﬀerence can be especially signiﬁcant at early ages when the
large macropores dictate the tensile response of concrete.
A comparison between the tensile modulus of concrete
and the corresponding mortar specimens are provided
in Figure 11.The results indicate that the concrete tensile
modulus is always higher than the mortar modulus due to
the stiﬀness provided by the coarse aggregates in concrete.
However,the diﬀerence is narrowed as concrete ages due to
hydration of cement which results in an increased stiﬀness of
the mortar.
15
20
25
30
35
40
15
20
25
30
35
40
0 1 2 3 4 5 6 7 8
Et
(GPa)
Ec
(GPa)
Age (day)
O57,tensileO57,compressive
O39,tensileO39,compressive
O25,tensileO25,compressive
Figure 10:Young’s moduli versus age of concrete.
15
20
25
30
35
40
15
20
25
30
35
40
0
1 2 3 4 5 6 7 8
MortarEt
(GPa)
ConcreteEt
(GPa)
Age (day)
O57,mortar
O39,mortar
O25,mortar
O57,concrete
O39,concrete
O25,concrete
Figure 11:Tensile Young’s modulus predicted by employing grids
of diﬀerent ﬁneness.
Advances in Civil Engineering 7
23
24
25
26
27
28
29
10
×
10
20
×
20
30
×
30
40
×
40
50
×
50
60
×
60
70
×
70
80
×
80
90
×
90
100
×
100
PredictedEt
(GPa)
Mesh size
E
m
:19 GPa
E
g
:36 GPa
V
a
:4.5%
V
g
:37.7%
Average
10
∼
100
10
∼
100
Figure 12:Comparison of experiment and predicted tensile
Young’s modulus.
5.Prediction of the Tensile
Young’s Modulus at Early Age
5.1.Input Data for Development of the Simpliﬁed Composite
Model.The tensile Young’s moduli of coarse aggregates
and mortar are needed as input parameters for use in the
composite models.While the moduli of mortar is directly
measured (Figure 11),it is diﬃcult to directly obtain the
tensile modulus of the aggregate due the size and number
of specimens required for tensile testing,diﬃculty in using a
proper tensile grip method of the rock specimen,as well as
the variability in the material properties due to layering and
impurities of the rock.Thus,the tensile Young’s modulus of
the coarse aggregate is indirectly calculated by employing the
Counto and Hashin models in the present study.The study
estimates the tensile Young’s modulus (E
g
) of 36.0 GPa from
the experimental result of O25 at age of 7 days,for which
the modulus of mortar was almost equal to the modulus of
concrete.That is,the estimated value to the modulus is little
aﬀected by the models used for obtaining the modulus of the
aggregate.Similar values are obtained based on testing O25
at earlier ages or by testing the other two mixtures.
Table 4 provides the input data for the composite model.
The volume fractions of each component (mortar,coarse
aggregates,and air) are obtained from the mix proportions
given in Table 3.To determine the appropriate number
of elements in the model,the study estimates the tensile
Young’s moduli of concrete by employing models of various
mesh sizes.Figure 12 presents the resulting tensile moduli
predicted as a function of mesh ﬁneness.The graph shows
the maximum,minimum,and average moduli obtained
from 10 consecutive simulations in each model.Based on
these results,a 80
×
80 model was chosen for the remaining
simulations in this work.
5.2.Quality of the Model Predictions.Figure 13 shows the
tensile Young’s moduli of all concrete specimens predicted
by using the proposed composite model.Each bar presents
the average of 10 simulations for each concrete mixture
and at each age.The bar graph indicates that the predicted
0.6
0.7
0.8
0.9
1
1.1
15
20
25
30
35
40
O57(2)
O57(3)
O57(7)
O57(28)
O39(1)
O39(2)
O39(3)
O39(7)
O25(1)
O25(2)
O25(3)
O25(7)
Et
(GPa)
Ratio
Ratio (experiment/predicted)
Experiment
Predicted
Figure 13:Tensile Young’s modulus predicted by employing grids
of diﬀerent ﬁneness.
15
20
25
30
35
40
1.5 2.5 3.5 4.5
Et
ofmortar(GPa)
E
t
(7)
=
4.3C/W+18.1
E
t
(1)
=
4.3C/W+7.9
E
t
(2)
=
4.3C/W+11.9
C/W
E
t
(3)
=
4.3C/W+15.2
Figure 14:Relations between cementwater ratio and tensile
Young’s moduli of mortar.
Young’s moduli are in good agreement with the experimental
values;the ratio of the two is in range of 0.90 to 1.07.This
implies that the tensile modulus of concrete can be predicted
appropriately by employing the composite model when the
volume fraction of constituents is known.
5.3.Empirical Formula for the Tensile Modulus of Mortars
in This Study.Considering that the Young’s modulus of
coarse aggregate and air content of concrete are age
independent,the Young’s modulus of concrete at early age
may be predicted if the modulus of mortar can be estimated
appropriately.For the mortar studied in this work,empirical
correlations between the experimental measurement mod
ulus,the W/C,and the age of mortars are established as
presented in Figure 14.The ﬁgure shows a linear correlation
between the inverse water to cement ratio (C/W) and the
tensile moduli of mortar (E
t
) at ages of 1,2,3,and 7 days.
Interestingly,the slope k
i
of all regression lines in the graph
is approximately 4.3 GPa:
Relation of E
t
−
C
W
:E
t
=
k
i
∙
C
W
+C
i
,(5)
where E
t
(GPa) is the tensile modulus of mortar,and C
i
(GPa) is an agedependent parameter in each regression line.
8 Advances in Civil Engineering
Table 4:Input data for the composite model.
Mix.ID V
m
V
g
V
a
E
t
of mortar (GPa) shown in Figure 11
E
g
(GPa)
1 day 2 days 3 days 7 days
O57 57.7% 37.7% 4.5% N/A 19.0 22.4 25.6 36.0
O39 62.0% 34.2% 3.8% 20.0 24.2 27.0 30.0 36.0
O25 66.4% 30.0% 3.6% 23.7 29.1 32.3 35.3 36.0
7.9
11.9
15.2
18.1
6
8
10
12
14
16
18
20
22
0 1 2 3 4 5 6 7 8 9 10
CoeﬃcientCi
(GPa)
Age T (day)
E
t
(T)
=
4.3C/W+C
i
R
=
0.93
C
i
(T)
=
21T
T
+1.5
Figure 15:Coeﬃcient C
i
of the regression line versus age of mortar.
The change in C
i
with age of mortar is shown in Figure 15.A
Goral curve [16],which is often used for estimating concrete
strength development with age,is ﬁt to the data points
resulting in the following:
Coeﬃcient C
i
with age:C
i
=
21T
T +1.5
,(6)
where T is mortar age in days.Combining (5) and (6) results
in
Tensile Young’s modulus of mortar:
E
t
(
T
)
=
4.3
C
W
+
21T
T +1.5
,
(7)
where E
t
is the estimated tensile Young’s modulus of mortar
(GPa).
It must be noted that similar to modulus of concrete,
the tensile modulus of mortar is a function of the volume
fraction and stiﬀness of sand,volume fraction and modulus
of cement paste (itself a function of age and W/C),and
the air content of the mortar.By accounting for age and
W/C,(7) can provide an estimate for the tensile modulus
of mortars with similar volume fraction and stiﬀness of
the ﬁne aggregates.Young’s modulus of coarse aggregate
can be considered as an inﬂuencing factor to the tensile
modulus of concrete,so this equation including the eﬀect of
ﬁne aggregate may be useful for normal concrete using sea
sand when an appropriate value of the modulus for coarse
aggregate is provided.To be applicable to mortars other than
those used here,the most signiﬁcant remaining parameter
is the volume fraction of sand which must be taken into
consideration.
5.4.Prediction of the Tensile Modulus of Concrete by the
Composite Model.By combining (7) with the composite
15
20
25
30
35
40
15 20 25 30 35 40
Prediction(GPa)
Experiment (GPa)
Present study
Aoki
Xie and Liu
Swadddiwdhipong
+15%
−
15%
Figure 16:Comparison of experiments and predictions.
model (Figure 6),the agedependent tensile moduli of
concrete can be estimated from its mixture proportions
(i.e.,volume fraction of constituents) and the aggregate
modulus.Figure 16 presents a comparison between the
model predictions and the experimental data fromthis study
as well as those fromprevious investigations [2,4,7].Herein,
these predicted data were obtained with the assumption that
the aggregate properties in other studies are equal to the
values employed in this study,because the modulus of coarse
aggregate used is not reported in the previous investigations.
The ﬁgure shows that the proposed method can predict the
tensile modulus of concrete,with reasonable accuracy,solely
based on the mixture proportions.
Figure 17(a) describes characteristics of tensile moduli of
concrete with W/C
=
55%and coarse aggregates of diﬀerent
volume fractions.The vertical axis in the graph presents the
tensile Young’s moduli ratio of concrete to coarse aggregate.
Herein,the model results are obtained fromthe assumptions
shown in Table 5.The ﬁgure demonstrates that the tensile
modulus of concrete increases with increasing the volume of
coarse aggregates since the aggregates have a higher Young’s
modulus than the mortars.It is also noted that tensile moduli
of concrete having more coarse aggregates (i.e.,larger vol.
fractions) than the solid volume content of coarse aggregates
[17] are unavailable.Figure 17(b) presents a similar set of
curves corresponding to concrete with W/C
=
30%.Both
ﬁgures describe that the tensile modulus of concrete develops
rapidly at early age and gradually plateaus at later ages.
Advances in Civil Engineering 9
Table 5:Conditions for simulation of tensile Young’s modulus.
Composite model See Figure 6
Elements 80
×
80
Air content 4.5%
Tensile Young’s modulus of mortar see (7)
Tensile Young’s modulus of coarse aggregate 36 GPa
Solid volume content of coarse aggregate 60%
Tensile Young’s modulus of concrete
Average of 10
simulations
40
50
60
70
80
90
100
0 20 40 60 80 100
28 d
3 d
1 d
2 d
5 d
7 d
14 d
91 d
Solid volume percentage
W/C:55%
V
a
:4.5%
RatioofEt
(conc./coarseagg.)
(%)
Volume of coarse aggregate
(%)
(a)
40
50
60
70
80
90
100
0 20 40 60 80 100
28 d
3 d
1 d
2 d
5 d
7 d
14 d
91 d
Solid volume percentage
W/C:30%
V
a
:4.5%
RatioofEt
(conc./coarseagg.)
(%)
Volume of coarse aggregate
(%)
(b)
Figure 17:Prediction results for tensile Young’s modulus of
concrete:(a) W/C
=
55%and (b) W/C
=
30%.
6.Conclusions
This paper describes the experimental measurement of
tensile Young’s modulus of concrete at early age using a direct
tension setup.Moreover,a predictive composite model was
developed to estimate the agedependent tensile modulus
of concrete using the volume fractions and properties of
the constituents.The main conclusions are summarized as
follows.
(1) The tensile stressstrain response of concrete was
observed to be very linear even at early ages (e.g.,1
day old).The residual strains after repeated loading
of specimens up to strains of 60
×
10
−
6
were neg
ligible.The tensile Young’s modulus obtained from
the stressstrain response develops according to the
watercement ratio and the age of concrete.
(2) The tensile modulus of concrete is approximately
1.0–1.3times larger than its compressive modulus
within the material’s ﬁrst week of age.As such,
estimation of the tensile modulus based on empirical
correlations with the compressive strength of con
crete can be inaccurate.
(3) The agedependent tensile moduli of concrete could
be predicted appropriately by the proposed com
posite model as long as the volume fractions of
coarse aggregates,mortar,and air,and the modulus
of aggregates are known.In comparison with the
experimental results,the model predictions showed
accuracy better than
±
15%.
References
[1] A.M.Neville,Properties of Concrete:Fourth and Final Edition,
Pearson/Prentice Hall,1995.
[2] Y.Aoki,K.Shimano,D.Iijima,and Y.Hirano,“Examination
on simple uniaxial tensile test of concrete,” Proceedings of the
Japan Concrete Institute,vol.29,no.1,pp.531–536,2007
(Japanese).
[3] Architectural Institute of Japan,Recommendations of Practice
of Crack Control in Reinforced Concrete BuildingsDesign and
Construction,Architectural Institute of Japan,2006.
[4] N.Xie and W.Liu,“Determining tensile properties of mass
concrete by direct tensile test,” ACI Materials Journal,vol.86,
no.3,pp.214–219,1989.
[5] F.A.Oluokun,E.G.Burdette,and J.H.Deatherage,“Elastic
modulus,Poisson’s ratio,and compressive strength relation
ships at early ages,” ACI Materials Journal,vol.88,no.1,pp.
3–10,1991.
[6] S.Hagihara,S.Nakamura,Y.Masuda,and M.Kono,“Exper
imental study on mechanical properties and creep behavior
of highstrength concrete in early age,” Concrete Research and
Technology,vol.11,no.1,pp.39–50,2000 (Japanese).
[7] S.Swaddiwudhipong,H.R.Lu,and T.H.Wee,“Direct tension
test and tensile strain capacity of concrete at early age,” Cement
and Concrete Research,vol.33,no.12,pp.2077–2084,2003.
[8] B.Bissonnette,M.Pigeon,and A.M.Vaysburd,“Tensile creep
of concrete:study of its sensitivity to basic parameters,” ACI
Materials Journal,vol.104,no.4,pp.360–368,2007.
[9] I.Yoshitake,Y.Ishikawa,H.Kawano,and Y.Mimura,“On
the Tensile Young’s Moduli of early age concrete,” Journal of
Materials,Concrete Structures and Pavements,vol.63,no.4,
pp.677–688,2007 (Japanese).
[10] T.J.Hirsh,“Modulus of elasticity of concrete aﬀected by elastic
moduli of cement paste matrix and aggregate,” ACI Journal,
vol.59,no.3,pp.427–452,1962.
[11] U.J.Counto,“The eﬀect of the elastic modulus of the
aggregate on the elastic modulus,creep and creep recovery of
concrete,” Magazine of Concrete Research,vol.16,pp.129–138,
1964.
[12] Z.Hashin,“The elastic moduli of heterogeneous materials,”
Journal of Applied Mechanics,ASME,vol.29,no.1,pp.143–
150,1962.
[13] H.Mihashi and J.P.D.B.Leite,“Stateoftheart report on
control of cracking in early age concrete,” Journal of Advanced
Concrete Technology,vol.2,no.2,pp.141–154,2004.
10 Advances in Civil Engineering
[14] F.P.Zhou,F.D.Lydon,and B.I.G.Barr,“Eﬀect of coarse
aggregate on elastic modulus and compressive strength of high
performance concrete,” Cement and Concrete Research,vol.25,
no.1,pp.177–186,1995.
[15] I.B.Topc¸u,“Alternative estimationof the modulus of elasticity
for damconcrete,” Cement and Concrete Research,vol.35,no.
11,pp.2199–2202,2005.
[16] L.M.Goral,“Empirical timestrength relations of concrete,”
ACI Journal,vol.53,pp.215–224,1956.
[17] JIS A 1104,“Methods of Test for Bulk Density of Aggregates
and Solid Content in Aggregates,” Japan Industrial Standards
Committee,2006.
Submit your manuscripts at
http://www.hindawi.com
Control Science
and Engineering
Journal of
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
International Journal of
Rotating
Machinery
Hindawi Publishing Corporation
http://www.hindawi.com
Volume 2013
Part I
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Distributed
Sensor Networks
International Journal of
ISRN
Signal Processing
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Mechanical
Engineering
Advances in
Modelling &
Simulation
in Engineering
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Advances in
OptoElectronics
Hindawi Publishing Corporation
http://www.hindawi.com
Volume 2013
ISRN
Sensor Networks
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
VLSI Design
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
The Scientific
World Journal
ISRN
Robotics
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
International Journal of
Antennas and
Propagation
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
ISRN
Electronics
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Journal of
Sensors
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Active and Passive
Electronic Components
Chemical Engineering
International Journal of
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Electrical and Computer
Engineering
Journal of
ISRN
Civil Engineering
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Advances in
Acoustics &
Vibration
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Comments 0
Log in to post a comment